- Nano Express
- Open Access
Substrate-Free InGaN/GaN Nanowire Light-Emitting Diodes
© Neplokh et al. 2015
- Received: 21 July 2015
- Accepted: 3 November 2015
- Published: 17 November 2015
We report on the demonstration of substrate-free nanowire/polydimethylsiloxane (PDMS) membrane light-emitting diodes (LEDs). Metal-organic vapour-phase epitaxy (MOVPE)-grown InGaN/GaN core–shell nanowires were encapsulated into PDMS layer. After metal deposition to p-GaN, a thick PDMS cap layer was spin-coated and the membrane was manually peeled from the sapphire substrate, flipped upside down onto a steel holder, and transparent indium tin oxide (ITO) contact to n-GaN was deposited. The fabricated LEDs demonstrate rectifying diode characteristics. For the electroluminescence (EL) measurements, the samples were manually bonded using silver paint. The EL spectra measured at different applied voltages demonstrate a blue shift with the current increase. This shift is explained by the current injection into the InGaN areas of the active region with different average indium content.
- Light-emitting diodes
- Substrate-free devices Gallium nitride
Nitride light-emitting diodes (LEDs) have found numerous applications in our everyday life (general lighting, automotive headlamps, traffic signals, indicator lamps for electronic devices, etc.). Today, the market is dominated by two-dimensional devices based on thin film technology. To further boost the LED performance and to add new functionalities, three-dimensional nanomaterials have recently emerged [1, 2]. In particular, nitride high-aspect-ratio nanocrystals (referred to as nanowires (NWs)) allow to improve the material quality of the LED active region and to facilitate the light extraction . The NW LED core–shell structure geometry also allows growth on non-polar m-planes to avoid undesirable quantum-confined Stark effect (QCSE).
The attractive feature of the NWs is that they provide high tolerance for the growth on lattice-mismatched substrates (e.g. growth of high-quality nitride NWs on silicon [4, 5] or sapphire). The concept of the ‘NW substrate independence’ can be further extended by transferring the NWs to other substrates (including non-crystalline materials) in either planar [6–9] or vertical [10–13] architectures. In this way, the NWs are used independently from their growth substrate, which can potentially be recycled. New functionalities for LEDs can be imagined. For example, NW LEDs can be mounted on metallic layers for efficient heat sinking or LEDs of different colours can be integrated on the same holder. In particular, flexible NW devices can be fabricated using this approach .
The first demonstration of nanowire flexible LEDs has been done using ZnO nanowires grown in solution on plastic substrate  demonstrating the electroluminescence in the visible range. However, the direct growth on the plastic substrate imposes to use a low temperature and strongly limits the range of accessible materials and growth techniques. To achieve high-efficiency visible emission, it is advantageous to make use of InGaN NWs elaborated at high temperature following standard epitaxial methods. The NWs can then be reported to a different substrate for LED fabrication. Recently, the first substrate-free nitride NW LED has been demonstrated employing the NW transfer . The InGaN/GaN NWs were grown on a non-conventional Si/SiO2/graphene template, embedded into a polymer and separated from their growth substrate by wet etching of a sacrificial SiO2 layer . In this work, we propose a different fabrication approach based on a mechanical peel-off of the NWs with the method described in the literature [10, 16, 17], which does not require any sacrificial layer and thus facilitates the fabrication. Self-assembled core/shell NWs containing seven InGaN/GaN quantum wells (QWs) were grown by metal-organic vapour-phase epitaxy (MOVPE) on c-sapphire substrates. The NW structure was probed by cathodoluminescence evidencing two spectrally shifted emissions originating from the InGaN/GaN QWs located on the top polar minus c-plane and on the lateral non-polar m-plane facets. For the LED fabrication, the NWs were encapsulated into a polydimethylsiloxane (PDMS) layer and mechanically peeled from their growth substrate. The obtained NW/PDMS composite membrane was electrically contacted and fixed on a steel holder. The electrical characteristics of membrane NW LEDs presented a rectifying behaviour. The electroluminescence (EL) appeared starting from 5 V forward bias. The EL spectra exhibited two peaks at 412 and 466 nm, and the relative peak intensity changed with applied bias. In agreement with the cathodoluminescence mapping, this spectral behaviour is attributed to the current injection into the areas of the active InGaN/GaN QWs with different average In content located on the lateral and on the top NW facets.
Nanowire Growth and Device Fabrication
Thin free-standing composite membranes are rather difficult to manipulate since they are fragile and can easily roll up. Therefore, an additional PDMS cap layer (~0.5 mm thick, cured at 80 °C for 2 h) was deposited on the metal contact to be used as a mechanical support. It helps to peel off the structure from the sapphire substrate and prevents the peeled layer from rolling. After the mechanical lift-off of the nanowire/PDMS membrane, the sample was flipped upside down and put onto a steel holder for further processing and easy manipulation. Then, the second contact was deposited on the n-type GaN core bases of the NWs, which after the membrane flipping were located on its top part. The 100-nm-thick indium tin oxide (ITO) layer was deposited by sputtering through a shadow mask with an array of 0.5-mm-diameter circular openings . After that, the shadow mask was slightly shifted and the 5-nm Ti/15-nm Al/5-nm Ti/100-nm Au metal pads were deposited to achieve a partial overlap between the metal and ITO (Fig. 3b); the corresponding work function suits ohmic injection in the n-GaN . Thus, we obtain an array of LEDs, each consisting of a large number of parallel-connected NWs. The LEDs share the same bottom contact but can be addressed independently by their top metal pad.
To get access to the metal contact to p-GaN shells, which is between the 18-μm PDMS encapsulating layer and the 0.5-mm cap layer, the cap layer was mechanically released over a small area at the sample edge and a piece of aluminium foil was attached to the metallization with silver paint, as schematized in Fig. 3b. The ITO/metal contact to n-GaN NW base parts, which is accessible on the sample surface, was connected using metallic probes for the electrical characterizations. For EL spectroscopy, copper wires were manually attached to the metal pads using silver paint and a sharpened wooden toothpick since the composite NW/PDMS structure cannot stand the micro-bonding procedure.
The LED starts to luminesce at a forward bias of ~5 V with a working current in the order of 1 mA. This relatively high light-up voltage is attributed to the non-ohmic nature of the ITO contact to the moderately doped p-GaN shell. As previously reported in  for single NW LEDs, at low injection. the low energy peak is dominant. With increasing voltage, the short-wavelength peak increases faster than the long-wavelength peak. The short-wavelength peak becomes dominant at high injection (8 V, 10 mA). This relative intensity variation between the two peaks can be understood in terms of the redistribution of the injection current in the nanowire. The saturation current through the active region is exponentially dependent on the In content, and, for the mentioned difference in In content by several per cent, the saturation currents of the axial and radial active region parts are strongly different . The high saturation current in the In-rich part favours the preferential injection in this region. However, as the injection increases, the current spreading in the resistive p-GaN shell part starts to play an important role . The current is redistributed due to the potential drop in the shell, and the injection in the radial part of the active region, which in addition has a larger surface compared to the axial region, becomes favourable. It should also be noted that the radial QWs on the m-plane are expected to have less defects in comparison to the axial QWs due to their lower In content. This would also lead to the lower EL droop at higher currents for the m-plane QWs and therefore to a domination of the short-wavelength EL peak at high injection.
The increase of the injection current above 10 mA resulted in the LED failure. We believe that the device degradation is not caused by the NW structural degradation, but by the top contact failure, for which we observe a morphology change. This failure at a relatively low current can be attributed to the mechanical deformations of the soft PDMS layer and to the Joule heating. The degradation also can be caused by ion diffusion into polymer layer during current spreading in the ITO contact . In the future contact optimizations, this effect can be suppressed by creating a thin metal layer between ITO and PDMS layers . Alternative transparent contacts based on CVD-grown graphene layers can also be used .
The LED fabrication has been performed on several membranes showing good process reproducibility. EL measurements of the LED after 2-week storage in ambient air have not evidenced any device degradation.
Substrate-free NW LEDs have been fabricated using the polymer embedding and peel-off procedure. The devices show rectifying electrical behaviour and emission in the blue spectral range. Further improvement of the transparent contact would make these LEDs competitive with the NW LEDs fabricated on rigid crystalline substrates. The developed fabrication approach allows for sapphire substrate recycling, which is important for the LED cost reduction. In addition, the proposed LED architecture allows for the fabrication of flexible high-brightness LEDs in the blue spectral range provided that an appropriate flexible transparent contact is optimized.
This work has been partially financially supported by ANR ‘Inverstissement d’Avenir’ programmes ‘GaNeX’ (ANR-11-LABX-2014) and ‘NanoSaclay’ (ANR-10-LABX-0035), by ANR-14-CE26-0020-01 project ‘PLATOFIL’, by FP7 Marie Curie projects ‘Funprob’ and ‘NanoEmbrace’ (grant no. 316751), and by EU ERC project ‘NanoHarvest’ (grant no. 639052). A. Babichev acknowledges the support of RFBR (project no. 15-02-08282 А, no. 14-02-31485), and of the Scholarship of the President of the Russian Federation for young scientists and graduate students (grant no. SP-4716.2015.1). The device processing has been performed at CTU-IEF-Minerve technological platform, member of the Renatech RTB network.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Li S, Waag A (2012) GaN based nanorods for solid state lighting. J Appl Phys. doi:10.1063/1.3694674 Google Scholar
- Shirasaki Y, Supran GJ, Bawendi MG, Bulovic V (2013) Emergence of colloidal quantum-dot light-emitting technologies. Nat Photonics. doi:10.1038/nphoton.2012.328 Google Scholar
- Kang MS, Lee CH, Park JB, Yoo H, Yi GC (2012) Gallium nitride nanostructures for light-emitting diode applications. Nano Energy. doi:10.1016/j.nanoen.2012.03.005 Google Scholar
- Foltynski B, Giesen C, Heuken M (2015) Self-organized growth of catalyst-free GaN nano-and micro-rods on Si (111) substrates by MOCVD. Phys Status Solidi B. doi:10.1002/pssb.201451508 Google Scholar
- Salomon D, Dussaigne A, Lafossas M, Durand C, Bougerol C, Ferret P, Eymery J (2013) Metal organic vapour-phase epitaxy growth of GaN wires on Si (111) for light-emitting diode applications. Nanoscale Res Lett. doi:10.1186/1556-276X-8-61 Google Scholar
- Collet M, Salomon S, Klein NY, Seichepine F, Vieu C, Nicu L, Larrieu G (2014) Large-scale assembly of single nanowires through capillary-assisted dielectrophoresis. Adv Materials. doi:10.1002/adma.201403039 Google Scholar
- Lee CH, Kim DR, Zheng X (2011) Fabrication of nanowire electronics on nonconventional substrates by water-assisted transfer printing method. Nano Lett. doi:10.1021/nl201901z Google Scholar
- Son K, Lee DH, Yi J, Lee WW, Park WI (2011) Synthesis and transfer of Si nanowire arrays embedded in photo-sensitive polymer films for non-planar electronics. J Physics D App Phys. doi:10.1088/0022-3727/44/1/015501 Google Scholar
- Liu Z, Xu J, Chen D, Shen G (2015) Flexible electronics based on inorganic nanowires. Chem Soc Rev. doi:10.1039/C4CS00116H Google Scholar
- Plass KE, Filler MA, Spurgeon JM, Kayes BM, Maldonado S, Brunschwig BS, Atwater HA, Lewis NS (2009) Flexible polymer-embedded Si wire arrays. Adv Materials. doi:10.1002/adma.200802006 Google Scholar
- Spurgeon JM, Boettcher SW, Kelzenberg MD, Brunschwig BS, Atwater HA, Lewis NS (2010) Flexible, polymer-supported, Si wire array photoelectrodes. Adv Materials. doi:10.1002/adma.201000602 Google Scholar
- Reimer ME, Bulgarini G, Akopian N, Hocevar M, Bavinck MB, Verheijen MA, Bakkers EPAM, Kouwenhoven LP, Zwiller V (2012) Bright single-photon sources in bottom-up tailored nanowires. Nat Commun. doi:10.1038/ncomms1746 Google Scholar
- Anttu N, Abrand A, Asoli D, Heurlin M, Aberg I, Samuelson L, Borgstroem M (2014) Absorption of light in InP nanowire arrays. Nano Res. doi:10.1007/s12274-014-0442-y Google Scholar
- Nadarajah A, Word RC, Meiss J, Könenkamp R (2008) Flexible inorganic nanowire light-emitting diode. Nano Lett. doi:10.1021/nl072784l Google Scholar
- Chung K, Beak H, Tchoe Y, Oh H, Yoo H, Kim M, Yi GC (2014) Growth and characterizations of GaN micro-rods on graphene films for flexible light emitting diodes. Appl Mater. doi:10.1063/1.4894780 Google Scholar
- Park S, Kim H, Vosgueritchian M, Cheon S, Kim H, Hoon Koo J, Kim TR, Lee S, Schwartz G, Chang H, Bao Z (2014) Stretchable energy-harvesting tactile electronic skin capable of differentiating multiple mechanical stimuli modes. Adv Materials. doi:10.1002/adma.201402574 Google Scholar
- Park KT, Guo Z, Um HD, Jung JY, Yang JM, Lim SK, Kim YS, Lee JH (2011) Optical properties of Si microwires combined with nanoneedles for flexible thin film photovoltaics. Opt Express. doi:10.1364/OE.19.000A41 Google Scholar
- Koester R, Hwang JS, Durand C, Dang DLS, Eymery J (2010) Self-assembled growth of catalyst-free GaN wires by metal–organic vapour phase epitaxy. Nanotechnology. doi:10.1088/0957-4484/21/1/015602 Google Scholar
- Koester R, Hwang JS, Salomon D, Chen X, Bougerol C, Barnes JP, Le Si DD, Rigutti L, Tchernycheva M, Durand C, Eymery J (2011) M-plane core–shell InGaN/GaN multiple-quantum-wells on GaN wires for electroluminescent devices. Nano Lett. doi:10.1021/nl202686n Google Scholar
- Tchoulfian P, Donatini F, Levy F, Dussaigne A, Ferret P, Pernot J (2014) Direct imaging of p–n junction in core–shell GaN wires. Nano Lett. doi:10.1021/nl5010493 Google Scholar
- PATENT Chen X, Durand C, Eymery J, Salomon D (2012). Process for catalyst-free selective growth on a semiconductor structure. patent number: WO2012136665.Google Scholar
- Befahy S, Yunus S, Burguet V, Heine JS, Troosters M, Bertrand P (2008) Stretchable gold tracks on flat polydimethylsiloxane (PDMS) rubber substrate. J of Adhesion. doi:10.1080/00218460801954292 Google Scholar
- Sheu JK, Su YK, Chi GC, Koh PL, Jou MJ, Chang CM, Liu CC, Hung WC (1999) High-transparency Ni/Au ohmic contact to p-type GaN. App Phys Lett. doi:10.1063/1.123844 Google Scholar
- Kalaitzakis FG, Pelekanos NT, Prystawko P, Leszczynski M, Konstantinidis G (2007) Low resistance as-deposited Cr/Au contacts on p-type GaN. App Phys Lett. doi:10.1063/1.2828044 Google Scholar
- Sheu JK, Su YK, Chi GC, Jou MJ, Liu CC, Chang CM (1999) Indium tin oxide ohmic contact to highly doped n-GaN. Solid State Electron. doi:10.1016/S0038-1101(99)00177-X Google Scholar
- Wang DF, Shiwei F, Lu C, Motayed A, Jah M, Mohammad SN, Jones KA, Salamanca-Riba L (2001) Low-resistance Ti/Al/Ti/Au multilayer ohmic contact to n-GaN. J Appl Phys. doi:10.1063/1.1350617 Google Scholar
- Jacopin G, De Luna BA, Lavenus P, Rigutti L, Julien FH, Zagonel LF, Kociak M, Durand C, Salomon D, Chen XJ, Eymery J, Tchernycheva M (2012) Single-wire light-emitting diodes based on GaN wires containing both polar and nonpolar InGaN/GaN quantum wells. Appl Phys Express. doi:10.1143/APEX.5.014101 Google Scholar
- Davydov VY, Klochikhin AA, Emtsev VV, Kurdyukov DA, Ivanov SV, Vekshin VA, Bechstedt F, Furthmueller J, Aderhold J, Graul J, Mudryi AV, Harima H, Hashimoto A, Yamamoto A, Haller EE (2002) Bandgap of hexagonal InN and InGaN alloys. Phys Status Solidi B. doi:10.1117/12.511325 Google Scholar
- Durand C, Bougerol C, Carlin JF, Rossbach G, Godel F, Eymery J, Jouneau P, Mukhtarova A, Butte R, Grandjean N (2014) M-Plane GaN/InAlN multiple quantum wells in core–shell wire structure for UV emission. ACS Photonics. doi:10.1021/ph400031x Google Scholar
- Hong YJ, Lee CH, Yoon A, Kim M, Seong HK, Chung HJ, Sone C, Park YJ, Yi GC (2011) Visible-color-tunable light-emitting diodes. Adv Mater. doi:10.1002/adma.201100806 Google Scholar
- Tchernycheva M, Lavenus P, Zhang H, Babichev AV, Jacopin G, Shahmohammadi M, Julien FH, Ciechonski R, Vescovi G, Kryliouk O (2014) InGaN/GaN core–shell single nanowire light emitting diodes with graphene-based p-contact. Nano Lett. doi:10.1021/nl5001295 Google Scholar
- Wang X, Zhi L, Muellen K (2008) Transparent, conductive graphene electrodes for dye-sensitized solar cells. Nano Lett. doi:10.1021/nl072838r Google Scholar
- Chang KM, Chu JY, Cheng CC (2004). Highly reliable GaN-based light-emitting diodes formed by p-In0.1Ga0.9N-ITO structure. Photonics Technology Letters. doi: 10.1109/LPT.2004.830523.
- Babichev AV, Zhang H, Lavenus P, Julien FH, Egorov AY, Lin YT, Tu LW, Tchernycheva M (2013) GaN nanowire ultraviolet photodetector with a graphene transparent contact. Appl Phys Lett. doi:10.1063/1.4829756 Google Scholar